- 197 Views
- Updated On :
- Presentation posted in: General

Chapter 9. Design for Sheet Metalworking. OutLine. 9.1 INTRODUCTION 9.2 DEDICATED DIES AND PRESSWORKING 9.2.1 Individual Dies for Profile Shearing 9.2.2 Cost of Individual Dies 9.2.3 Individual Dies for Piercing Operations 9.2.4 Individual Dies for Bending Operations

Chapter 9

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Chapter 9

Design for Sheet Metalworking

Dr. Mohammad Abuhaiba

9.1 INTRODUCTION

9.2 DEDICATED DIES AND PRESSWORKING

9.2.1 Individual Dies for Profile Shearing

9.2.2 Cost of Individual Dies

9.2.3 Individual Dies for Piercing Operations

9.2.4 Individual Dies for Bending Operations

9.2.5 Miscellaneous Features

9.2.6 Progressive Dies

9.3 PRESS SELECTION

9.3.1 Cycle Times

9.4 TURRET PRESS WORKING

9.5 PRESS BRAKE OPERATIONS

9.6 DESIGN RULES

Dr. Mohammad Abuhaiba

Parts are made from sheet in two ways:

- Dies to
- Make blanks
- change shape of blanks
- add features through piercing operations

- CNC punching machines
- arrays of sheet metal parts from individual sheets.
- punches in rotating turrets (turret presses)

Dr. Mohammad Abuhaiba

- Stiffness per unit cost in sheet form is max for steels

Dr. Mohammad Abuhaiba

Dr. Mohammad Abuhaiba

A sheet metal part is produced through a series of shearing and forming operations.

- Individual dies on separate presses
- Progressive die: different stations within a single die.
- Strip is moved incrementally through die while press cycles.
- punches at different positions along die produce successive features in part.

Dr. Mohammad Abuhaiba

Dr. Mohammad Abuhaiba

- applies to parts that have two parallel edges & "jigsaw" together along length of strip.
- Trailing edge of part must be precise inverse of leading edge

Dr. Mohammad Abuhaiba

Advantages:

- Simple tooling
- Minimization of manufactured scrap.
- Manufactured scrap: scrap sheet metal produced as a direct result of the manufacturing process.

Dr. Mohammad Abuhaiba

- Sheet metal part designed with two parallel edges, but ends cannot jigsaw together.
- Two die blocks and a punch passing between them to remove material separating ends of adjacent parts.
- Sheared ends should not meet strip edges at an angle less than about 15° to ensure a good-quality sheared edge with a min of tearing & edge distortion at ends of cut.
- Avoid Full semicircular ends or corner blend radii

Dr. Mohammad Abuhaiba

- Part-off process offers same advantage as cut-off
- Die is a little more complex than a cutoff die.

Dr. Mohammad Abuhaiba

- Scrap is increased because adjacent parts must be separated by at least twice sheet metal thickness to allow adequate punch strength.

Dr. Mohammad Abuhaiba

- parts do not have two straight parallel edges.
- Blank can be almost any closed contour.
- Increase in mfg scrap.
- Edges of part must be separated from edges of strip by nearly twice sheet metal thickness to minimize edge distortion.

Dr. Mohammad Abuhaiba

- Extra scrap area / part = 4 × material thickness × part length
- Blanking dies are more expensive to produce than cut-off or part-off dies.
- Additional plate, stripper plate, positioned above die plate with separation sufficient to allow sheet metal strip to pass between.
- Stripper plate aperture matches contour of punch so that it uniformly supports strip while punch is removed from it on upward stroke of press.

Dr. Mohammad Abuhaiba

- If both ends are symmetric, then adjacent parts can be arranged on strip at a 180° orientation to each other.
- Each press stroke produces two parts.

Dr. Mohammad Abuhaiba

- A rounded edge on the die side of part from initial deformation as sheet is pressed downward against die edge.
- Final separation of part from strip is by brittle fracture, which leaves a sharp edge, or burr, on punch side of part.
- Sharp edges on opposite sides of adjacent parts.
- De-burring: sharp edges must be removed: tumbling

Dr. Mohammad Abuhaiba

- For each type of die the cost includes a basic die set:
- Cds = die set purchase cost, $
- Au = usable area between guide pillars, cm2

Dr. Mohammad Abuhaiba

- Mfg point system to estimate cost of tooling elements such as:
- die plate
- Punch
- punch retaining plate
- stripper plate, etc.

- The system includes time for:
- mfg die elements
- Assembly
- tryout of die

- Assembly includes custom work on die set:
- drilling and tapping of holes
- fitting of metal strips or dowel pins to guide sheet metal stock in die

Dr. Mohammad Abuhaiba

- Basic mfg points are determined by:
- size of punch
- complexity of profile to be sheared

- Profile complexity is measured by index Xpas
- P = perimeter length to be sheared, cm
- L,W = length & width of smallest rectangle surrounding the punch, cm

Dr. Mohammad Abuhaiba

- L and W:
- Blanking die, or a cut-off and drop-through die: length & width of smallest rectangle surrounding the entire part.
- Part-off die: L is distance across strip while W is width of zone removed from between adjacent parts.
- Cut-off die: L and W are dimensions of a rectangle surrounding end contour of part.

- for either cut-off or part-off, min punch width W of about 6 mm should be allowed to ensure sufficient punch strength.

Dr. Mohammad Abuhaiba

Dr. Mohammad Abuhaiba

- Basic point score is multiplied by a correction factor for the plan area of punch

Dr. Mohammad Abuhaiba

- Basic manufacturing points:
- Part-off die: 9% less than for blanking
- Cut-off die: 12% less than for blanking
- For die mfg, where CNC wire EDM is used to cut the necessary profiles in:
- die blocks
- punch blocks
- punch holder plates
- stripper plates

- each mfg point in Fig. 9.9 corresponds to one equivalent hour of die making.

Dr. Mohammad Abuhaiba

- This includes time for cutting, squaring, & grinding required tool steel blocks & plates.
- Estimated point score from Figs. 9.9 & 9.10 does not include effect of:
- thicker-gage sheet metal
- higher-strength sheet metal
- very large production volumes of parts

Dr. Mohammad Abuhaiba

- Recommendations on die plate thickness hdfit quite well with the relationship
- U = ultimate tensile stress of sheared sheet metal
- Ums = ultimate tensile stress of annealed mild steel
- V = required production volume, thousands
- h = sheet metal thickness, mm
- value of hdis usually rounded to nearest one eighth of an inch to correspond with standard tool steel stock sizes.

Dr. Mohammad Abuhaiba

- Mfg points in Fig. 9.9 were determined for the condition
- Or hd = 25 mm
- cost of dies changes with die plate thickness according to a thickness factor fd:
- Or fd = 0.75 Whichever is the larger.

Dr. Mohammad Abuhaiba

Mfgpoints Mp for a blanking die:

- Mpo= basic mfg points (Fig. 9.9)
- f1w= plan area correction factor (Fig. 9.10)
- fd = die plate thickness correction factor (Eq. 9.5)

Dr. Mohammad Abuhaiba

Example

- A sheet metal blank 200mm long by 150mm wide, plain semicircular ends with radius 75 mm.
- 500,000 parts, 16 gage low carbon steel.
- Estimate cost of a blanking die to produce part and % of manufactured scrap.

Dr. Mohammad Abuhaiba

Example

- Required blank area =200 x150 mm2.
- 50mm space is allowed around part for securing of die plate & installation of strip guides
- Required die set usable area Auis
Au = (20 + 2 x 5) x (15 + 2 x 5) = 750 cm2

- Eq 9.1: cost of die set
Cds = 120 + (0.36 x 750) = $390

Dr. Mohammad Abuhaiba

Example

- Perimeter of Required blanking punch, P = 571 mm
- L, W = 150 and 200 mm
- Perimeter complexity index Xp=5712/(150x200) = 10.9
- Basic mfg point score (Fig. 9.9), Mpo = 30.5
- plan area LW = 300 cm2
- correction factor (Fig. 9.10) = 2.5

Dr. Mohammad Abuhaiba

Example

- For 500,000 parts of thickness 1.52mm , die plate thickness (Eq 9.3) hd= 26.6 mm
- Die plate thickness correction factor (Eq. 9.5) fd=1.03
- Total die mfg points Mp=1.03x2.5x30.5=78.5 hour
- $40/h for die making
- Blanking die cost = 390+78.5x40 = $3530

Dr. Mohammad Abuhaiba

Example

- Area of each part Ap = 251.7 cm2
- Separation between each part on strip and between part and strip edges should be 3.04mm (twice material thickness),
- area of sheet used for each part, As =(200+3.04) x (150 +2 x 3.04) mm2 = 316.9 cm2
- Scrap % = (316.9 - 251.7)/316.9 x 100 = 20.6

Dr. Mohammad Abuhaiba

Example

- If part were redesigned with 80mm radius ends (Fig. 9.11b), it could then be produced with a part-off die. What would be die cost and % of mfg scrap for this case?
- perimeter to be sheared = length of two 80 mm arcs = P = 388.9mm
- With 3.04mm separating parts end to end on strip: L, W of part-off punch =106.5 and 150mm

Dr. Mohammad Abuhaiba

Example

- Complexity index Xp = 388.92/(106.5 x 150) = 9.5
- part plan area = 300 cm2 , mfg points are the same as for blanking die.
- part-off dies are 9% less expensive than blanking dies for same Cpx value, and values of fd and f1ware unchanged, total die mfg hours are
- M = 0.91 x 1.03 x 2.5 x 30.5 = 71.4
- $40/h for die making
- Part-off die cost = 390 + 71.4 x 40 = $3,250

Dr. Mohammad Abuhaiba

Example

- Area of each part = 257.9 cm2
- edges of strip correspond to edges of part
- area of sheet used for each part As= (200 + 3.04) x 150 mm2 = 304.6 cm2
- Scrap % = (304.6 - 257.9)/304.6 x 100 = 15.3

Dr. Mohammad Abuhaiba

- A piercing die: same as blanking die except that material is sheared by punching action to produce internal holes or cut-outs in the blank.
- Piercing dies: several punches
- Individual punch areas have only a minor effect on final die cost.
- Main cost drivers:
- number of punches
- size of part
- perimeter length of cutting edges of any nonstandard punches.

Dr. Mohammad Abuhaiba

- Nonstandard punch: cross-sectional shape other than circular, square, rectangular, or obround
- Mfg point score: three main components
- Based only on area of part to be pierced, base manufacturing score is:
- L, W = length & width of rectangle enclosing all holes to be punched, cm

Dr. Mohammad Abuhaiba

- Eq 9.7 predicts number of hours to mfg:
- basic die block
- punch retaining plate
- stripper plate
- die backing plate

- This must be added to time to mfg punches and to produce corresponding apertures in die block.
- This time depends upon:
- number of required punches
- total perimeter of punches

Dr. Mohammad Abuhaiba

- Mfg time Mpc for custom punches
- Pp = total perimeter of all punches, cm
- Np = number of punches
- Eq 9.8: estimates time to mfg nonstandard punches & for cutting corresponding die apertures

Dr. Mohammad Abuhaiba

- Standard punch shapes (Fig. 9.12):
- Mfg hours, Mps for standard punches and die inserts, and for time to cut appropriate holes in punch retaining plate and die plate:
- K = 1 for round holes
- K = 3.5 for square, rectangular, or obround holes
- Np = number of punches
- Nd = number of different punch shapes and sizes

Dr. Mohammad Abuhaiba

- Determine cost of piercing die to punch three holes.
- Rectangle that surrounds the three holes has dimensions 120 x 90 mm
- nonstandard "C“ shaped hole has a perimeter length equal to 260mm.

Dr. Mohammad Abuhaiba

- Base mfg score (Eq. 9.7) = Mpo= 23 + 0.03(12 x 9) = 26 h
- Number of hours required to mfg custom punching elements for nonstandard aperture (Eq 9.8)
Mpc = 8 + 0.6 x 26 + 3 = 26.6 h

- Equivalent mfg time for punches, die plate inserts, etc., for the two "standard" circular holes (Eq 9.9)
Mps = 2 x 2 + 0.4 x 1 = 4.4 h

- 50 mm space is allowed around part in die set
- required plate area = Au = (20+2 x 5) x (10+2 x 5) = 600 cm2
- die set cost = $336
- Estimated piercing die cost, assuming $40/h for die making = 336 + (26 + 26.6 + 4.4) x 40 = $2,616

Dr. Mohammad Abuhaiba

Bends are typically produced by one of two die-forming methods:

- V-die and punch combination (Fig. 9.14a)
- Least expensive type of bending die
- difficulty of precisely positioning metal blank and a resulting lack of precision in bent part

- Greater control of bend location on part

Dr. Mohammad Abuhaiba

- U-die (double-wiper die)
- Z-die (double v-die)

Dr. Mohammad Abuhaiba

part shown can be formed in a single die.

- a z-die first forms front step.
- Lower die block then proceeds to move downward against spring pressure so that stationary wiper blocks adjacent to the three other sides displace the material upward.

Dr. Mohammad Abuhaiba

In order to determine number of separate bending dies required for a particular part, apply the following rules:

- Bends that lie in the same plane, such as the four bends surrounding the central area in Fig. 9.16, can usually be produced in one die.
- Secondary reverse bends in displaced metal, such as lower step in Fig. 9.16, can often be produced in the same die using a z-die action.
- Secondary bends in displaced metal that would lead to a die-locked condition will usually be produced in a separate die.

Dr. Mohammad Abuhaiba

- Bends a, c, and d or bends a, b, and d could be formed in one die by a combination of a wiper die and a z-die.
- Remaining bend would then require a 2nd wiper die and a separate press operation.
- Bend b could be produced in the 2nd die using a tooling arrangement (Fig. 9.18).

Dr. Mohammad Abuhaiba

- Bend b could be produced in the 2nd die using a tooling arrangement (Fig. 9.18).

Dr. Mohammad Abuhaiba

Cost of bending dies:

- A point score related to tool mfg hours.
- Based on area of flat part to be bent and final depth of bent part, the base die mfg score for bending is:
- L,W = length & width of rectangle surrounding part, cm
- D = final depth of bent part, cm, or 5.0, whichever is larger

Dr. Mohammad Abuhaiba

- Additional number of points are added for length of bend lines to be formed and for number of separate bends to be formed simultaneously:
- Lb= total length of bend lines, cm
- Nb = number of different bends to be formed in die
- Cost of a die set must be added according to Eq. 9.1

Dr. Mohammad Abuhaiba

Example

- Fig. 9.16: Part is produced from a flat blank 44cm long by 24cm wide.
- Five bends
- Total length of bend lines = 76 cm
- Height of formed part from top edge of box to bottom of step = 12cm
- Eq. 9.10: Mpo= [18+0.023x(44 x 24)]x(0.88+0.02 x 12) =42.3x1.12 = 47.4h
- Additional points for bend length & multiple bends:
Mpn= 0.68 x 76 + 5.8 x 5 = 80.7 h

- 5.0 cm clearance around part in die set, then cost of die set is estimated from Eq. 9.1
Cds = 120 + 0.36 x (54 x 34) = $780

- $40/h for tool making
- cost of bending die: Cd= 780 + (47.4 + 80.7) x 40 = $5900

Dr. Mohammad Abuhaiba

- A lance: cut in sheet metal part that is required for an internal forming operation.
- Cutting edges of punch are pressed only partway through the material thickness, sufficient to produce the required shear fracture.

Dr. Mohammad Abuhaiba

- Depressions: localized shallow-formed regions produced by pressing sheet downward into a depression in the die plate with a matching profile punch.
- Beads: Patterns of long, narrow depressions onto the open surfaces of sheet metal parts in order to increase bending stiffness.
- In a depression sheet material reduces in thickness as a result of being stretched around the punch profile.

Dr. Mohammad Abuhaiba

- Depression on left side of part (Fig. 9.19), assume material is stretched by around 15% in every direction.
- Because volume of metal stays constant after forming, thickness will have been reduced by nearly 30%.
- Embossed region on right side of part (Fig. 9.19) is reduced in thickness by direct compression between punch and die.

Dr. Mohammad Abuhaiba

- Hole flanges: produced by pressing a taper or bullet-nosed cylindrical punch into a smaller punched hole.
- Material is stretched by entry of larger punch and displaced in direction of punch travel.
- Due to ductility limitations: flanged height = 2 to 3 *sheet metal thickness

Dr. Mohammad Abuhaiba

- Cost of dies for these miscellaneous operations can be determined from equations for costs of piercing dies.
- Eq 9.7 : determine base cost of die plates, punch blocks, etc.
- Eq. 9.8: Additional cost of punch and die machining
- Parameter Pp = perimeter of forming or cutting punches
- Number Mpx of additional hours of punch and die machining is
- Nsp = total number of separate surface patches to be machined on punch faces and matching die surfaces

Dr. Mohammad Abuhaiba

- Multi-station die on a single press.
- Stations within die carry out different piercing, forming, & shearing operations as sheet metal is transported incrementally through die.

Dr. Mohammad Abuhaiba

- For complex-shaped parts, perimeter will usually be sheared in increments at different stations with only final parts of profile being sheared at last station.
- More uniform distribution of shearing forces among different stations, resulting in balanced loads on die.
- Bending operations to be performed with wiper dies when portions of perimeter around bend have been removed.

- Two additional holes in strip (Fig. 9.20) are punched at 1st station & then engaged with taper-nosed punches at 2nd station.
- more precise registration between stations so that part accuracy does not depend on accuracy of strip feeding mechanism.

Dr. Mohammad Abuhaiba

Cpd = 2Cid (9.13)

- Cpd = cost of single progressive die
- Cid = cost of individual dies for blanking, cut-off or part-off, piercing, and forming operations for the same part
- Factor of 2: moderate complex parts
- Factor of 3: very complex parts
- Factor of 1.5: very simple parts

Dr. Mohammad Abuhaiba

- Required force f for: blanking, piercing, lancing, etc., is given by
- h = gage thickness, m
- ls = length to be sheared, m

Dr. Mohammad Abuhaiba

Example: circular disks 50 cm in diameter are to be blanked from No. 6 gage commercial-quality, low-carbon steel.

- (Tables 9.1 & 9.2):
- thickness of 6 gage steel = 5.08 x 10-3m
- ultimate tensile strength, U = 330 x103kN/m2

- required blanking force f = 0.5 x (330 x 103) x (5.08 x 10-3) x (px 50 x 10-2) = 1316.6kN
- Table 9.3: 1750kN press

Dr. Mohammad Abuhaiba

Bending or shallow forming operations:

- required forces are usually much less than for shearing.
- Fig. 9.22: assume inside bend radius, r = 2*h

Dr. Mohammad Abuhaiba

Under these conditions, as material is bent around die profile, through increasing angle q:

- length of outer surface increases to 3hq.
- length of centerline of material (neutral axis) remains nearly constant at 2.5hq.
- strain in outer fibers of material is:
- strain decreases to zero from outer fibers to centerline, and then becomes compressive, increasing to nearly -0.2 on inside surface.

Dr. Mohammad Abuhaiba

- average strain in bent material = 0.5e
- work done per unit volume on material as it forms around die = stress * strain
- assume that punch radius = 2 * thickness
- 90° bend: punch moves down, while in contact with part, through a distance of ~5h.
- volume of material subjected to bending is
- Lb= bend length

Dr. Mohammad Abuhaiba

- energy balance:
- f = average press force that moves through distance 5h
- Eary and Reed [4] give an empirical relationship for wiper die bending as
- r1= profile radius of punch
- r2 = profile radius of die

Dr. Mohammad Abuhaiba

Shallow forming (Fig. 9.19): vertical resisting force from walls is

- L = perimeter of depression.
- for a depression with vertical walls (q=90°) required punch force can approach twice force required to shear material around perimeter.

Dr. Mohammad Abuhaiba

Fig. 9.19: required force for an embossing operation is

- A = area to be embossed
- F = constraint factor > 1
- As size of embossed region increases, factor F increases exponentially.

Dr. Mohammad Abuhaiba

Ostwald, time to:

- load a blank or part into a mechanical press,
- operate the press, and
- remove part following the press operation

- L, W = rectangular envelope length & width, cm
- Apply 2/3 of time given by Eq 9.22 for shearing or piercing of flat parts (automatic press ejection)

Dr. Mohammad Abuhaiba

Fig. 9.20: compare cycle times and processing costs for using individual dies to those for progressive die working. Part is made from No. 8 gage stainless steel.

- Ultimate tensile stress = 515MN/m2
- Outer perimeter of part = 370 mm
- thickness = 4.17mm
- Eq 9.14: required shear force for blanking outer perimeter, f1 =0.5x(515x103)x(4.17x370 x10-6)= 397kN
- For piercing obroundcutout with perimeter 149mm, required force, f2= 160 kN

Dr. Mohammad Abuhaiba

- Force required for bending tab across ~25 mm bend line, with assumed 6mm tool profile radii, is given from Eq. (9.19) as
f3 =0.333x515x103x(25x10-3)x(4.172x10-6/((6+6)x10-3)= 6.2kN

- Table 9.3: blanking operation would require 500 kN press, and piercing and bending operations could be carried out on the smallest 200 kN press.

Dr. Mohammad Abuhaiba

Individual Dies

- For blanking and piercing operations: assume automatic ejection of blanks and scrap.
- cycle time for these two operations will be 2/3 of time for loading and unloading given by Eq. (9.22):
t1 = 0.67 x (3.8 + 0.11(10 + 11.5)) = 0.67 x 5.4 = 3.6s

- For bending operation, part unloading is required:
t2 = 5.4 s

- Table 9.3: press hourly rates
- processing cost per part, Cp= [(3.6/3600)x76 + (3.6/3600)x55 + (5.4/3600) x 55] x 100 cents = 21.4 cents

Dr. Mohammad Abuhaiba

Progressive Die

- required press force, f = f1 +f2 +f3 = 563 kN
- space required for four die stations = 4 x 100 + 3(2 x 4.17) = 418.5 mm
- Table 9.3: press has:
- press force = 1750 kN
- operating cost =105 $/h
- press speed = 35 strokes/min

- estimated cycle time per part = t = 60/35 = 1.7s
- processing cost per part, Cp= (1.7/3600) x 105 x 100 = 5.0 cents

Dr. Mohammad Abuhaiba

- For parts that are to be manufactured with dedicated dies, design outer profile with parallel straight edges defining part width.
- To allow for satisfactory shearing in cut-off or part-off operations, end profiles should meet straight edges at angles no less than 15°.

Dr. Mohammad Abuhaiba

- No narrow projections or notches that will require narrow weak sections in either punches or die plates (dimensions marked "a" in Fig. 9.27)

Dr. Mohammad Abuhaiba

- Avoid Small holes or narrow cut-outs that will require fragile punches.
- Internal punched holes should be separated from each other, and from outside edge, with sufficient clearance to avoid distortion of narrow sections of work-piece material during punching.

Dr. Mohammad Abuhaiba

- Both feature dimensions and feature spacings should be at least twice material thickness.
- Fig. 9.27, satisfactory blanking and punching will require that dimensions labeled "a" through "d" should all be greater than or equal to twice gage thickness.

Dr. Mohammad Abuhaiba

- "e“, corner radii in die plate: Radii equal to at least twice gage thickness will minimize corner stress concentrations in die plate, which may lead to crack formation and failure.

Dr. Mohammad Abuhaiba

- Incorporate relief cut-outs dimensioned as "d," at ends of proposed bend lines that terminate at internal corners in outer profile.
- If for any reason holes that intersect outer profile must be punched later, then diameter should be at least three times gage thickness to accommodate offset loading to which punch will be subjected.

Dr. Mohammad Abuhaiba

- When formed features are being considered, principal design constraint is max tensile strain the material can withstand (Table 9.2).
- Fig. 9.28:
- component made from low-carbon, commercial-quality steel
- Transition from surface to top of bridge = 45°.

Dr. Mohammad Abuhaiba

Dr. Mohammad Abuhaiba

- Assuming uniform stretching of bridge, tensile strain along bridge is
- If max permissible strain in tension is 0.22 (Table 9.2), then from Eq. (9.29) successful forming will be assured if
- Length of bridges > 4 times height
- For different materials or varying geometries, tensile strains must be estimated & compared to permissible max value.

Dr. Mohammad Abuhaiba

Louver (Figure 9.29):

- Length of front edge must be greater than a certain multiple of louver opening height H, determined by material ductility and end ramp angles exactly as in the bridge calculation.

Dr. Mohammad Abuhaiba

- Stretching also occurs at right angles to louver edge where material is stretched upward into a circular arc.
- This will not cause material failure, since front edge of louver will be pulled backward as tensile stress develops in the surface.
- Choice of radius R (Fig. 9.29) is more one of appearance and amount of space taken up by a single louver.

Dr. Mohammad Abuhaiba

- Hole flanging: provide increased local thickness for tapping of screw threads
- Hole flange is formed by pressing a taper-nosed punch of diameter D into a smaller punched hole of diameter d.
- Tensile strain around top edge of formed flange is

Dr. Mohammad Abuhaiba

- e < permissible material ductility
- Typical values of flange height in sheet steel components range between 2 and 3 times material gage thickness.

Dr. Mohammad Abuhaiba

- Ribs may be circular V-shaped.
- For a required height, H, width and shape of rib must be chosen so that required amount of stretching across rib does not exceed material ductility.

- Radius at base of rib must be greater than a certain value to prevent overstraining material on underside of part.

Dr. Mohammad Abuhaiba

- Max tensile strain in bending is in the outer fibers of the sheet on the outside of the bend and is governed by the ratio of inside bend radius, r, to sheet gage thickness, h.
- For a bend through any angle q, length of outer surface is
- length of surface in center of sheet (neutral axis) is
- strain on outer surface is
- Radius r is defined precisely by profile radius of bending tool:
- convex radius of die block for a wiper die
- convex radius of punch in a v-die.

Dr. Mohammad Abuhaiba

- Min acceptable radius value can be obtained from Eq. (9.34) and ductility of material to be bent.
- Example: low-carbon, commercial-quality steel with ductility 0.22, Eq. (9.34) gives
- Inside bend radius ≥ twice sheet thickness (limiting value for a material with 20% ductility)

Dr. Mohammad Abuhaiba

- Fig. 9.32: slots would almost certainly have to be punched after the bending operation.
- This is because small separation, l, of edges of slots from bend line would result in distortion of slots during bending if they were punched first.

Dr. Mohammad Abuhaiba

- If part contains other holes or slots that are now on nonparallel surfaces to the one shown, then two separate dies and operations are needed for punching where one would otherwise have been sufficient.
- Edge of circular holes should preferably be 2 times sheet thickness from beginning of a bend.
- For slots parallel to a bend this clearance should increase to 4 times sheet thickness.

Dr. Mohammad Abuhaiba

- Blanked parts or punched holes with max dimensions up to 10cm can be held to tolerances of around ±0.05 mm
- As part size increases, precision is more difficult to control
- For a part with dimensions as large as 50 cm permissible tolerances are in the range of ±0.5 mm.
- For formed parts, or formed features, variation tends to be larger and minimum tolerances attainable are in the range of ±0.25 mm for small parts.
- A tight tolerance between punched holes, which are on parallel surfaces separated by bends, would require holes to be punched after bending at greater expense.
- If holes are on nonparallel surfaces, then machining may be necessary to obtain required accuracy.

Dr. Mohammad Abuhaiba

- nesting
- If individual dies are to be used, then part should be designed if possible for cut-off or part-off operations.
- Figure 9.33:
- cut-off design lacks elegance of rounded end profiles.
- acute sharp corner will be removed during debarring

Dr. Mohammad Abuhaiba